29th May, 2017
When selecting a stick electrode, consider the base metal type, joint fit-up and welding positions. Before you begin welding consider the below.
Determine your base metal composition. Your goal is to closely match the electrode composition to the base metal type, this will help ensure a strong weld.
To prevent cracking or other weld issues, match the minimum tensile strength of the electrode to the base metal. To identify this, refer to the first two digits of the AS/NZS classification (see figure 1). For example, the number “43” on a 4313 electrode indicates that the filler metal produces a weld bead with a minimum tensile strength of 430Mpa, meaning it would work well with a steel of similar tensile strength.
Some electrodes can be used with only AC or DC power sources while other electrodes are compatible with both. To determine the correct current type, refer to the second two digits of the AS/NZS classification (see figure 1), which represents the type of coating and type of compatible welding current (see figure 2).
For example, an E4916 electrode can be used in the flat, horizontal, vertical and overhead positions (all).
The type of current you use also influences the penetration profile of the weld. For example, a DCEP compatible electrode, such as an E4310 delivers deep penetration and produces an extremely tight arc. It also can “dig” through rust, oil, paint and dirt. A DCEN compatible electrode, such as an E4312, provides mild penetration and works well when bridging two joints or welding high speed, high current fillet welds in the horizontal position.
An AC compatible electrode, such as an E4313, produces a soft arc with medium penetration and should be used to weld clean, new sheet metal.
Thick materials require an electrode with maximum ductility and low hydrogen to prevent weld cracking. Electrodes with AS/NZS classification numbers ending in 15, 16 or 18 provide excellent low–hydrogen properties and good toughness (high impact values) to accommodate for residual stress.
For thin materials, you will need an electrode that produces soft arcs, such as a 4313. Also, smaller diameter electrodes will provide shallow penetration to help prevent burn-through on thinner materials.
If you’re working on a joint with a tight fit-up or one that is not bevelled, use an electrode that provides a digging arc to ensure sufficient penetration, such as an E4310 or E4311. For materials with wide root openings, E4312 electrodes, creates a concave weld face suitable for bridging gaps and making groove welds.
For high heat or low temperature environments, subjected to repetitive shock loading, a low hydrogen electrode with higher ductility will reduce the chance of cracking. Also, check for welding specifications. If you’re working on critical applications, it’s likely a specific type of electrode will need to be used.
For best results, clean your base metal, this will help prevent porosity and increase travel speeds. If not possible, E4310 or E4311 electrodes deliver a deep penetrating arc that can cut through contaminants.
SHOP STICK ELECTRODES FROM WIA